Plywood - wikipedia Plywood This article needs additional citations for verification. Please help improve this article by adding citations to reliable sources. Unsourced material may be challenged and removed. ( June 2013 ) Softwood plywood made from spruce Plywood is a sheet material manufactured from thin layers or `` plies '' of wood veneer that are glued together with adjacent layers having their wood grain rotated up to 90 degrees to one another. It is an engineered wood from the family of manufactured boards which includes medium - density fibreboard ( MDF ) and particle board ( chipboard ). All plywoods bind resin and wood fibre sheets ( cellulose cells are long, strong and thin ) to form a composite material. This alternation of the grain is called cross-graining and has several important benefits : it reduces the tendency of wood to split when nailed in at the edges ; it reduces expansion and shrinkage, providing improved dimensional stability ; and it makes the strength of the panel consistent across all directions. There is usually an odd number of plies, so that the sheet is balanced -- this reduces warping. Because plywood is bonded with grains running against one another and with an odd number of composite parts, it has high stiffness perpendicular to the grain direction of the surface ply. Smaller, thinner, and lower quality plywoods may only have their plies ( layers ) arranged at right angles to each other. Some better quality plywood products will by design have five plies in steps of 45 degrees ( 0, 45, 90, 135, and 180 degrees ), giving strength in multiple axes. Contents 1 Etymology 2 History 3 Structural characteristics 4 Types 4.1 Softwood plywood 4.2 Hardwood plywood 4.3 Tropical plywood 4.4 Aircraft plywood 4.5 Decorative plywood ( overlaid plywood ) 4.6 Flexible plywood 4.7 Marine plywood 4.8 Other plywoods 5 Production 6 Sizes 7 Grades 8 Applications 8.1 Softwood plywood applications 8.2 Hardwood plywood applications 8.3 Tropical plywood applications 9 References 10 External links Etymology The word `` Ply '' derives from the French verb plier, `` to fold '', from the Latin verb plico, from the ancient Greek verb πλέκω. History In 1797 Samuel Bentham applied for patents covering several machines to produce veneers. In his patent applications, he described the concept of laminating several layers of veneer with glue to form a thicker piece -- the first description of what we now call plywood. Bentham was a British naval engineer with many shipbuilding inventions to his credit. Veneers at the time of Bentham were flat sawn, rift sawn or quarter sawn ; i.e. cut along or across the log manually in different angles to the grain and thus limited in width and length. About fifty years later Immanuel Nobel, father of Alfred Nobel, realized that several thinner layers of wood bonded together would be stronger than one single thick layer of wood understanding the industrial potential of laminated wood he invented the rotary lathe. There is little record of the early implementation of the rotary lathe and the subsequent commercialization of plywood as we know it today, but in its 1870 edition, the French dictionary Robert describes the process of rotary lathe veneer manufacturing in its entry Déroulage. One can thus presume that rotary lathe plywood manufacture was an established process in France in the 1860s. Plywood was introduced into the United States in 1865 and industrial production started shortly after. In 1928, the first standard - sized 4 ft by 8 ft ( 1.2 m by 2.4 m ) plywood sheets were introduced in the United States for use as a general building material. Artists use plywood as a support for easel paintings to replace traditional canvas or cardboard. Ready - made artist boards for oil painting in three - layered plywood ( 3 - ply ) were produced and sold in New York as early as 1880. In India, plywood is more commonly called `` Kitply '' after a leading brand which pioneered the concept of waterproof plywood in the early 1970 's Structural characteristics A typical plywood panel has face veneers of a higher grade than the core veneers. The principal function of the core layers is to increase the separation between the outer layers where the bending stresses are highest, thus increasing the panel 's resistance to bending. As a result, thicker panels can span greater distances under the same loads. In bending, the maximum stress occurs in the outermost layers, one in tension, the other in compression. Bending stress decreases from the maximum at the face layers to nearly zero at the central layer. Shear stress, by contrast, is higher in the center of the panel, and at the outer fibres. Types Average - quality plywood with ' show veneer ' High - quality concrete pouring plate in plywood Birch plywood Different varieties of plywood exist for different applications : Softwood plywood Softwood plywood is usually made either of cedar, Douglas fir or spruce, pine, and fir ( collectively known as spruce - pine - fir or SPF ) or redwood and is typically used for construction and industrial purposes. The most common dimension is 1.2 by 2.4 metres ( 3 ft 11 in × 7 ft 10 in ) or the slightly larger imperial dimension of 4 feet × 8 feet. Plies vary in thickness from 1.4 mm to 4.3 mm. The number of plies -- which is always odd -- depends on the thickness and grade of the sheet. Roofing can use the thinner 5 / 8 '' ( 15 mm ) plywood. Subfloors are at least 3 / 4 '' ( 18 mm ) thick, the thickness depending on the distance between floor joists. Plywood for flooring applications is often tongue and groove ; This prevents one board from moving up or down relative to its neighbor, providing a solid - feeling floor when the joints do not lie over joists. T&G plywood is usually found in the 1 / 2 '' to 1 '' ( 12 -- 25 mm ) range. Hardwood plywood Hardwood plywood is made out of wood from angiosperm trees and used for demanding end uses. Hardwood plywood is characterized by its excellent strength, stiffness and resistance to creep. It has a high planar shear strength and impact resistance, which make it especially suitable for heavy - duty floor and wall structures. Oriented plywood construction has a high wheel - carrying capacity. Hardwood plywood has excellent surface hardness, and damage - and wear - resistance. Tropical plywood Tropical plywood is made of mixed species of tropical wood. Originally from the Asian region, it is now also manufactured in African and South American countries. Tropical plywood is superior to softwood plywood due to its density, strength, evenness of layers, and high quality. It is usually sold at a premium in many markets if manufactured with high standards. Tropical plywood is widely used in the UK, Japan, United States, Taiwan, Korea, Dubai, and other countries worldwide. It is an excellent choice for construction purposes in many regions due to its low cost. However, many countries ' forests have been over-harvested, including the Philippines, Malaysia and Indonesia, largely due to the demand for plywood production and export. Aircraft plywood De Havilland DH - 98 Mosquito was made of curved and glued veneers High - strength plywood, also known as aircraft plywood, is made from mahogany, spruce and / or birch using adhesives with an increased resistance to heat and humidity. It was used in the construction of air assault gliders during World War II and also several fighter aircraft, most notably the multi-role British Mosquito. Nicknamed `` The Wooden Wonder '' plywood was used for the wing surfaces, and also flat sections such as bulkheads and the webs of the wing spars. The fuselage had exceptional rigidity from the bonded ply - balsa - ply ' sandwich ' of its monocoque shell ; elliptical in cross-section, it was formed in two separate mirror - image halves, using curved moulds. Structural aircraft - grade plywood is most commonly manufactured from African mahogany, spruce or birch veneers that are bonded together in a hot press over hardwood cores of basswood or poplar or from European Birch veneers throughout. Basswood is another type of aviation - grade plywood that is lighter and more flexible than mahogany and birch plywood but has slightly less structural strength. Aviation - grade plywood is manufactured to a number of specifications including those outlined since 1931 in the Germanischer Lloyd Rules for Surveying and Testing of Plywood for Aircraft and MIL - P - 607, the latter of which calls for shear testing after immersion in boiling water for three hours to verify the adhesive qualities between the plies and meets specifications. Decorative plywood ( overlaid plywood ) Usually faced with hardwood, including ash, oak, red oak, birch, maple, mahogany, Philippine mahogany ( often called lauan, luan or meranti and having no relation to true mahogany ), rosewood, teak and a large number of other hardwoods. Flexible plywood Flexible plywood is designed for making curved parts, a practice which dates back to the 1850s in furniture making. Aircraft grade plywood, often Baltic birch, is made from 3 or more plies of birch, as thin as 1 / 64 '' thick in total, and is extremely strong and light. At 3 / 8 '' thick, mahogany 3 - ply `` wiggle Board '' or `` Bendy Board '' come in 4 ' x 8 ' sheets with a very thin cross grain central ply and two thicker exterior plies, either long grain on the sheet, or cross grain. Wiggle board is often glued together in two layers once it is formed into the desired curve, so that the final shape will be stiff and resist movement. Often, decorative wood veneers are added as a surface layer. In the UK single ply sheets of veneer were used to make stovepipe hats in Victorian times, so flexible modern plywood is sometimes known there as `` Hatters Ply '', although the original material was not strictly plywood, but a single sheet of veneer. Marine plywood Marine plywood is manufactured from durable face and core veneers, with few defects so it performs longer in both humid and wet conditions and resists delaminating and fungal attack. Its construction is such that it can be used in environments where it is exposed to moisture for long periods. Each wood veneer will be from tropical hardwoods, have negligible core gap, limiting the chance of trapping water in the plywood and hence providing a solid and stable glue bond. It uses an exterior Water and Boil Proof ( WBP ) glue similar to most exterior plywoods. Marine plywood can be graded as being compliant with BS 1088, which is a British Standard for marine plywood. There are few international standards for grading marine plywood and most of the standards are voluntary. Some marine plywood has a Lloyd 's of London stamp that certifies it to be BS 1088 compliant. Some plywood is also labeled based on the wood used to manufacture it. Examples of this are Okoumé or Meranti. Other plywoods Other types of plywoods include fire - retardant, moisture - resistant, wire mesh, sign - grade, and pressure - treated. However, the plywood may be treated with various chemicals to improve the plywood 's fireproofing. Each of these products is designed to fill a need in industry. Baltic Birch plywood is a product of an area around the Baltic Sea. Originally manufactured for European cabinet makers but now popular in the United States as well. It is very stable composed of an inner void - free core of cross-banded birch plys with an exterior grade adhesive. The face veneers are thicker than traditional cabinet grade plywood. Production Logs for plywood construction in a plywood factory Plywood production requires a good log, called a peeler, which is generally straighter and larger in diameter than one required for processing into dimensioned lumber by a sawmill. The log is laid horizontally and rotated about its long axis while a long blade is pressed into it, causing a thin layer of wood to peel off ( much as a continuous sheet of paper from a roll ). An adjustable nosebar, which may be solid or a roller, is pressed against the log during rotation, to create a `` gap '' for veneer to pass through between the knife and the nosebar. The nosebar partly compresses the wood as it is peeled ; it controls vibration of the peeling knife ; and assists in keeping the veneer being peeled to an accurate thickness. In this way the log is peeled into sheets of veneer, which are then cut to the desired oversize dimensions, to allow it to shrink ( depending on wood species ) when dried. The sheets are then patched, graded, glued together and then baked in a press at a temperature of at least 140 ° C ( 284 ° F ), and at a pressure of up to 1.9 MPa ( 280 psi ) ( but more commonly 200 psi ) to form the plywood panel. The panel can then be patched, have minor surface defects such as splits or small knot holes filled, re-sized, sanded or otherwise refinished, depending on the market for which it is intended. Plywood for indoor use generally uses the less expensive urea - formaldehyde glue, which has limited water resistance, while outdoor and marine - grade plywood are designed to withstand moisture, and use a water - resistant phenol - formaldehyde glue to prevent delamination and to retain strength in high humidity. Anti-fungal additives such as Xyligen ( Furmecyclox ) may sometimes be added to the glueline to provide added resistance to fungal attack. The adhesives used in plywood have become a point of concern. Both urea formaldehyde and phenol formaldehyde are carcinogenic in very high concentrations. As a result, many manufacturers are turning to low formaldehyde - emitting glue systems, denoted by an `` E '' rating. Plywood produced to `` E0 '' has effectively zero formaldehyde emissions. In addition to the glues being brought to the forefront, the wood resources themselves are becoming the focus of manufacturers, due in part to energy conservation, as well as concern for natural resources. There are several certifications available to manufacturers who participate in these programs. Programme for the Endorsement of Forest Certification ( PEFC ) Forest Stewardship Council ( FSC ), Leadership in Energy and Environmental Design ( LEED ), Sustainable Forestry Initiative ( SFI ), and Greenguard are all certification programs that ensure that production and construction practices are sustainable. Many of these programs offer tax benefits to both the manufacturer and the end user. Sizes The most commonly used thickness range is from ⁄ to 3.0 inches ( 3.2 to 76.2 mm ). The sizes of the most commonly used plywood sheets are 4 x 8 feet ( 1220 x 2440 mm ) which was first used by the Portland Manufacturing Company, who developed what we know of as modern veneer core plywood for the 1905 Portland World Fair. A common metric size for a sheet of plywood is 1200 x 2400 mm. 5 × 5 feet ( 1,500 × 1,500 mm ) is also a common European size for Baltic birch ply, and aircraft ply. Sizes on specialised plywood for concrete - forming can range from ⁄ to ⁄ in ( 6 to 21 mm ), and a multitude of formats exist, though 15 × 750 × 1,500 mm (. 059 inch × 30 × 59 in ) ( 19 / 32in × 2 ft - 6in × 4 ft - 11in ) is very commonly used. Aircraft plywood is available in thicknesses of ⁄ inch ( 3 mm ) ( 3 ply construction ) and upwards ; typically aircraft plywood uses veneers of 0.5 mm ( approx 1 / 64 in ) thickness although much thinner veneers such as 0.1 mm are also used in construction of some of the thinner panels. Grades Grading rules differ according to the country of origin. The most popular standards are the British Standard ( BS ) and the American Standard ( ASTM ). Joyce ( 1970 ), however, list some general indication of grading rules : Grade Description Face and back veneers practically free from all defects. A / B Face veneers practically free from all defects. Reverse veneers with only a few small knots or discolorations. A / BB Face as A but reverse side permitting jointed veneers, large knots, plugs, etc. Both side veneers with only a few small knots or discolorations. B / BB Face veneers with only a few small knots or discolorations. Reverse side permitting jointed veneers, large knots, plugs, etc. BB Both sides permitting jointed veneers, large knots, plugs, etc. C / D For structural plywood, this grade means that the face has knots and defects filled in and the reverse may have some that are not filled. Neither face is an appearance grade, nor are they sanded smooth. This grade is often used for sheathing the surfaces of a building prior to being covered with another product like flooring, siding, concrete, or roofing materials. WG Guaranteed well glued only. All broken knots plugged. X Knots, knotholes, cracks, and all other defects permitted. WBP Weather and Boil Proof used in Marine Ply. Designation replaced by EN 314 - 3. JPIC Standards Grade Description BB / CC Face as BB, back as CC. BB as very little knots of less than 1 / 4 inches, slight discoloration, no decay, split and wormholes mended skillfully, matched colors, no blister, no wrinkle. Most popular choice for most applications. Applications Plywood is used in many applications that need high - quality, high - strength sheet material. Quality in this context means resistance to cracking, breaking, shrinkage, twisting and warping. Exterior glued plywood is suitable for outdoor use, but because moisture affects the strength of wood, optimal performance is achieved where the moisture content remains relatively low. Subzero conditions do not affect the dimensional or strength properties of plywood, making some special applications possible. Plywood is also used as an engineering material for stressed - skin applications. It has been used for marine and aviation applications since WWII. Most notable is the British de Havilland Mosquito bomber, with a fuselage made of birch plywood sandwiching a balsa core, and using plywood extensively for the wings. Plywood was also used for the hulls in the hard - chine Motor Torpedo Boats ( MTB ) and Motor Gun Boats ( MGB ) built by the British Power Boat Company and Vosper 's. Plywood is currently successfully used in stressed - skin applications. The American designers Charles and Ray Eames are known for their plywood - based furniture, as is Finnish Architect Alvar Aalto and his firm Artek, while Phil Bolger has designed a wide range of boats built primarily of plywood. Jack Köper of Cape Town designed the plywood Dabchick sailing dinghy, which as of 2015 is still sailed by large numbers of teenagers. Plywood is often used to create curved surfaces because it can easily bend with the grain. Skateboard ramps often utilize plywood as the top smooth surface over bent curves to create transition that can simulate the shapes of ocean waves. Softwood plywood applications Typical end uses of spruce plywood are : Floors, walls and roofs in home constructions Wind bracing panels Vehicle internal body work Packages and boxes Fencing There are coating solutions available that mask the prominent grain structure of spruce plywood. For these coated plywoods there are some end uses where reasonable strength is needed but the lightness of spruce is a benefit e.g. : Concrete shuttering panels Ready - to - paint surfaces for constructions Hardwood plywood applications Phenolic resin film coated ( Film Faced ) plywood is typically used as a ready - to - install component e.g. : Panels in concrete form work systems Floors, walls and roofs in transport vehicles Container floors Floors subjected to heavy wear in various buildings and factories Scaffolding materials ( `` Wire '' or other styles of imprinting available for better traction ) Birch plywood is used as a structural material in special applications e.g. : Wind turbine blades Insulation boxes for liquefied natural gas ( LNG ) carriers Smooth surface and accurate thickness combined with the durability of the material makes birch plywood a favorable material for many special end uses e.g. : High - end loud speakers Die - cutting boards Supporting structure for parquet Playground equipment Furniture Signs and fences for demanding outdoor advertising Musical instruments Sports equipment Tropical plywood applications Tropical plywood is widely available from the South - East Asia region, mainly from Malaysia and Indonesia. Tropical plywood boasts premium quality, and strength. Depending on machinery, tropical plywood can be made with high accuracy in thickness, and is a highly preferable choice in America, Japan, Middle East, Korea, and other regions around the world. Common plywood Concrete panel Floor base Structure panel Container flooring Lamin board Laminated veneer lumber ( LVL ) References Jump up ^ Collins Dictionary of the English Language, 2nd Edition, London, 1986, p. 1181 Jump up ^ Cassell 's Latin Dictionary, Marchant, J.R.V, & Charles, Joseph F., ( Eds. ), Revised Edition, 1928, p. 421 ^ Jump up to : `` Plywood ''. Gale 's How Products are Made. The Gale Group Inc. Retrieved 26 November 2013. Jump up ^ `` Nobel Plywood ''. Retrieved 2018 - 04 - 03. Jump up ^ `` Dérouler ''. Le Robert Historique de la langue française. Dictionnaires Robert. Retrieved 26 November 2013. Jump up ^ `` Plywood ''. Columbia Encyclopedia. Retrieved 26 November 2013. Jump up ^ Muller, Norman E. `` An early example of a plywood support for painting ''. Journal of the American Institute for Conservation. American Institute for Conservation of Historic and Artistic Works. Retrieved 26 November 2013. Jump up ^ O'Halloran, p. 221. Jump up ^ Handbook of Finnish plywood, Finnish Forest Industries Federation, 2002, ISBN 952 - 9506 - 63 - 5 `` Archived copy '' ( PDF ). Archived from the original ( PDF ) on 2007 - 09 - 27. Retrieved 2007 - 09 - 27. Jump up ^ Entry on the PAN Pesticide Database. Retrieved 8 June 2016. Jump up ^ Engineered Wood Products Association of Australasia. ( PDF ). Retrieved on 2012 - 02 - 10. Jump up ^ Pro Woodworking Tips.com. Pro Woodworking Tips.com. Retrieved on 2012 - 02 - 10. Jump up ^ Metric conversions, Canadian government publication Archived 2010 - 02 - 16 at the Wayback Machine... ( PDF ). Retrieved on 2012 - 02 - 10. Jump up ^ Joyce, Ernes. 1970. The Technique of Furniture Making. London : B.T. Batsford Limited. Jump up ^ http://www.supply5.co.za External links Look up plywood in Wiktionary, the free dictionary. APA -- The Engineered Wood Association Material Uses Pro Woodworking Tips.com Canadian Plywood Association Plywood Wood products Lumber / timber Batten Beam Bressummer Cruck Flitch beam Flooring Joist Lath Molding Panelling Plank Plate Post Purlin Rafter Railroad ties Reclaimed Shingle Siding Sill Stud Timber truss Treenail Truss Utility pole Engineered wood Glued laminated timber veneer LVL parallel strand I - joist Fiberboard hardboard Masonite MDF Oriented strand board Oriented structural straw board Particle board Plywood Structural insulated panel Wood - plastic composite lumber Fuelwood Charcoal biochar Firelog Firewood Pellet fuel Wood fuel Fibers Cardboard Corrugated fiberboard Paper Paperboard Pulp Pulpwood Rayon Derivatives Birch - tar Cellulose nano Hemicellulose Cellulosic ethanol Dyes Lignin Liquid smoke Lye Methanol Pyroligneous acid Pine tar Pitch Sandalwood oil Tannin Wood gas By - products Barkdust Black liquor Ramial chipped wood Sawdust Tall oil Wood flour Wood wool Woodchips Historical Axe ties Clapboard Dugout canoe Potash Sawdust brandy Split - rail fence Tanbark Timber framing Wooden masts See also Biomass Certified wood Destructive distillation Dry distillation Engineered bamboo Forestry List of woods Mulch Non-timber forest products Papermaking Wood drying Wood preservation Wood processing Woodworking Forestry portal Trees portal Commons WikiProject Forestry GND : 4155715 - 3 NDL : 00562527 Retrieved from `` https://en.wikipedia.org/w/index.php?title=Plywood&oldid=834504641 '' Categories : Plywood Engineered wood Composite materials Hidden categories : Webarchive template wayback links Articles needing additional references from June 2013 All articles needing additional references All articles with unsourced statements Articles with unsourced statements from December 2016 Articles with unsourced statements from April 2013 Articles with unsourced statements from November 2010 Articles with unsourced statements from November 2014 Articles with unsourced statements from April 2007 Articles containing potentially dated statements from 2015 All articles containing potentially dated statements Wikipedia articles with GND identifiers Talk Contents About Wikipedia Bân - lâm - gú Беларуская Беларуская ( тарашкевіца ) ‎ Български Boarisch Català Čeština Dansk Deutsch Eesti Español Esperanto فارسی Français Gàidhlig 한국어 Հայերեն हिन्दी Bahasa Indonesia Íslenska Italiano עברית Қазақша Lietuvių Magyar Nederlands 日本 語 Norsk Polski Português Română Русский Simple English Slovenčina Ślůnski Српски / srpski Suomi Svenska తెలుగు ไทย Türkçe Українська 中文 35 more Edit links This page was last edited on 6 April 2018, at 02 : 04. Text is available under the Creative Commons Attribution - ShareAlike License ; additional terms may apply. By using this site, you agree to the Terms of Use and Privacy Policy. Wikipedia ® is a registered trademark of the Wikimedia Foundation, Inc., a non-profit organization. About Wikipedia

Question: when did plywood start being used in furniture
Answer: the 1850s